LMucko/crystallography-open-database huggingface dataset:
Redetermination of the crystal structure of tetrasodium tetrahedro- tetrastannide, Na~4~Sn~4~ and tetrapotassium tetrahedro-tetrastannide, K~4~Sn~4~
Baitinger, M.; von Schnering, H. G.; Grin, Yu.; Kniep, R.; Zeitschrift für Kristallographie - New Crystal Structures 214 (1999) 453–454; doi:

data_8101629
_publ_section_title
;
Redetermination of the crystal structure of tetrasodium tetrahedro-
tetrastannide, Na~4~Sn~4~ and tetrapotassium tetrahedro-tetrastannide, 
K~4~Sn~4~
;
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              453
_journal_page_last               454
_journal_volume                  214
_journal_year                    1999
_chemical_formula_structural     'K4 Sn4'
_chemical_formula_sum            'K4 Sn4'
_chemical_formula_weight         5049.28
_chemical_name_common            'potassium stannide'
_space_group_IT_number           142
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4bd 2c'
_symmetry_space_group_name_H-M   'I 41/a c d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.409(1)
_cell_length_b                   11.409(1)
_cell_length_c                   18.649(2)
_cell_volume                     2427.5(7)
_diffrn_ambient_environment      air
_diffrn_ambient_temperature      295
_exptl_crystal_density_diffrn    3.4482(6)
_refine_ls_R_factor_obs          0.0360
_refine_ls_wR_factor_obs         0.0360
_cod_depositor_comments
;
 Changing the _atom_site_occupancy data item value from '.' to '1'
 for all fully occupied atom sites.

 Antanas Vaitkus,
 2017-02-10
;
_cod_original_sg_symbol_H-M      'I 41/a c d'
_cod_database_code               8101629
Crystal structure of tetrarubidium tetrahedro-tetraplumbide, Rb~4~Pb~4~ and of tetracaesium tetrahedro-tetraplumbide, Cs~4~Pb~4~
Baitinger, M.; Peters, K.; Somer, M.; von Schnering, H. G.; Carillo-Cabrera, W.; Grin, Yu.; Kniep, R.; Zeitschrift für Kristallographie - New Crystal Structures 214 (1999) 455–456; doi:

data_8101630
_publ_section_title
;
Crystal structure of tetrarubidium tetrahedro-tetraplumbide, Rb~4~Pb~4~ 
and of tetracaesium tetrahedro-tetraplumbide, Cs~4~Pb~4~
;
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              455
_journal_page_last               456
_journal_volume                  214
_journal_year                    1999
_chemical_formula_sum            'Pb4 Rb4'
_chemical_formula_weight         9365.12
_chemical_name_common            'Rubidium plumbide'
_space_group_IT_number           142
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4bd 2c'
_symmetry_space_group_name_H-M   'I 41/a c d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.892(1)
_cell_length_b                   11.892(1)
_cell_length_c                   19.429(2)
_cell_volume                     2747.6(8)
_diffrn_ambient_environment      air
_diffrn_ambient_temperature      295
_exptl_crystal_density_diffrn    5.6593(2)
_refine_ls_R_factor_obs          0.0375
_refine_ls_wR_factor_obs         0.0375
_cod_depositor_comments
;
 Changing the _atom_site_occupancy data item value from '.' to '1'
 for all fully occupied atom sites.

 Antanas Vaitkus,
 2017-02-10
;
_cod_original_sg_symbol_H-M      'I 41/a c d'
_cod_original_formula_sum        'Rb4 Pb4'
_cod_database_code               8101630
Crystal structure of tetrarubidium tetrahedro-tetrastannide, Rb~4~Sn~4~ and of tetracaesium tetrahedro-tetrastannide, Cs~4~Sn~4~
Baitinger, M.; Grin, Yu.; von Schnering, H. G.; Kniep, R.; Zeitschrift für Kristallographie - New Crystal Structures 214 (1999) 457–458; doi:

data_8101631
_publ_section_title
;
Crystal structure of tetrarubidium tetrahedro-tetrastannide, Rb~4~Sn~4~ 
and of tetracaesium tetrahedro-tetrastannide, Cs~4~Sn~4~
;
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              457
_journal_page_last               458
_journal_volume                  214
_journal_year                    1999
_chemical_formula_structural     'Rb4 Sn4'
_chemical_formula_sum            'Rb16 Sn16'
_chemical_formula_weight         6533.12
_chemical_name_common            'rubidium stannide'
_space_group_IT_number           142
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4bd 2c'
_symmetry_space_group_name_H-M   'I 41/a c d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   11.757(1)
_cell_length_b                   11.757(1)
_cell_length_c                   19.215(2)
_cell_volume                     2656.0(7)
_diffrn_ambient_environment      air
_diffrn_ambient_temperature      295
_exptl_crystal_density_diffrn    4.0797(6)
_refine_ls_R_factor_obs          0.0532
_refine_ls_wR_factor_obs         0.0532
_cod_depositor_comments
;
 Changing the _atom_site_occupancy data item value from '.' to '1'
 for all fully occupied atom sites.

 Antanas Vaitkus,
 2017-02-10
;
_cod_original_sg_symbol_H-M      'I 41/a c d'
_cod_database_code               8101631
Crystal structure of tetrarubidium tetrahedro-tetrastannide, Rb~4~Sn~4~ and of tetracaesium tetrahedro-tetrastannide, Cs~4~Sn~4~
Baitinger, M.; Grin, Yu.; von Schnering, H. G.; Kniep, R.; Zeitschrift für Kristallographie - New Crystal Structures 214 (1999) 457–458; doi:

data_8101632
_publ_section_title
;
Crystal structure of tetrarubidium tetrahedro-tetrastannide, Rb~4~Sn~4~ 
and of tetracaesium tetrahedro-tetrastannide, Cs~4~Sn~4~
;
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              457
_journal_page_last               458
_journal_volume                  214
_journal_year                    1999
_chemical_formula_structural     'Cs4 Sn4'
_chemical_formula_sum            'Cs16 Sn16'
_chemical_formula_weight         8051.2
_chemical_name_common            'Caesium stannide'
_space_group_IT_number           142
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4bd 2c'
_symmetry_space_group_name_H-M   'I 41/a c d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.122(1)
_cell_length_b                   12.122(1)
_cell_length_c                   19.820(2)
_cell_measurement_temperature    295
_cell_volume                     2912.4(8)
_diffrn_ambient_environment      air
_diffrn_ambient_temperature      295
_exptl_crystal_density_diffrn    4.5890(1)
_refine_ls_R_factor_obs          0.0671
_refine_ls_wR_factor_obs         0.0671
_cod_depositor_comments
;
 Changing the _atom_site_occupancy data item value from '.' to '1'
 for all fully occupied atom sites.

 Antanas Vaitkus,
 2017-02-10
;
_cod_original_sg_symbol_H-M      'I 41/a c d'
_cod_database_code               8101632
Crystal structure of alkaline earth dilithium bis(nitridolithiate/ferrates (I)), Ca{Li~2~[(Li~1-x~Fe~x~)N]~2~}, x = 0.30 and Sr{Li~2~[(Li~1-x~Fe~x~N)] ~2~}, x = 0.46
Klatyk, Jens; Kniep, Rüdiger; Zeitschrift für Kristallographie - New Crystal Structures 214 (1999) 449–450; doi:

data_8101633
_publ_section_title
;
Crystal structure of alkaline earth dilithium bis(nitridolithiate/ferrates
(I)), Ca{Li~2~[(Li~1-x~Fe~x~)N]~2~}, x = 0.30 and Sr{Li~2~[(Li~1-x~Fe~x~N)]
~2~}, x = 0.46
;
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              449
_journal_page_last               450
_journal_volume                  214
_journal_year                    1999
_chemical_formula_moiety         CaLi~2~[(Li~0.70~Fe~0.30~N]~2~
_chemical_formula_structural     'Ca Li2 [(Li0.70 Fe0.30 N]2'
_chemical_formula_sum            'Ca Fe0.61 Li3.39 N2'
_chemical_formula_weight         125.57
_space_group_IT_number           141
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4bd 2'
_symmetry_space_group_name_H-M   'I 41/a m d :2'
_cell_angle_alpha                90.000(7)
_cell_angle_beta                 90.000(8)
_cell_angle_gamma                90.00(9)
_cell_formula_units_Z            4
_cell_length_a                   3.7637(3)
_cell_length_b                   3.7637(4)
_cell_length_c                   26.168(3)
_cell_measurement_temperature    293(2)
_cell_volume                     370.68(6)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    2.250
_refine_ls_R_factor_obs          0.0184
_refine_ls_wR_factor_obs         0.0496
_cod_original_sg_symbol_H-M      'I 41/a m d'
_cod_original_formula_sum        'Ca Fe.61 Li3.39 N2'
_cod_database_code               8101633
Crystal structure of alkaline earth dilithium bis(nitridolithiate/ferrates (I)), Ca{Li~2~[(Li~1-x~Fe~x~)N]~2~}, x = 0.30 and Sr{Li~2~[(Li~1-x~Fe~x~N)] ~2~}, x = 0.46
Klatyk, Jens; Kniep, Rüdiger; Zeitschrift für Kristallographie - New Crystal Structures 214 (1999) 449–450; doi:

data_8101634
_publ_section_title
;
Crystal structure of alkaline earth dilithium bis(nitridolithiate/ferrates
(I)), Ca{Li~2~[(Li~1-x~Fe~x~)N]~2~}, x = 0.30 and Sr{Li~2~[(Li~1-x~Fe~x~N)]
~2~}, x = 0.46
;
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              449
_journal_page_last               450
_journal_volume                  214
_journal_year                    1999
_chemical_formula_sum            'Fe0.93 Li3.08 N2 Sr'
_chemical_formula_weight         188.64
_space_group_IT_number           141
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4bd 2'
_symmetry_space_group_name_H-M   'I 41/a m d :2'
_cell_angle_alpha                90.000(12)
_cell_angle_beta                 90.000(10)
_cell_angle_gamma                90.000(12)
_cell_formula_units_Z            4
_cell_length_a                   3.7909(2)
_cell_length_b                   3.7909(4)
_cell_length_c                   27.719(3)
_cell_measurement_temperature    293(2)
_cell_volume                     398.35(7)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    3.145
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Tetragonal' changed to 'tetragonal'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_sg_symbol_H-M      'I 41/a m d'
_cod_database_code               8101634
Crystal structure of dilithium (nitridolithiate/ferrate(I)), Li~2~ [(Li~1-x~Fe~x~)N], x = 0.63
Klatyk, Jens; Kniep, Rüdiger; Zeitschrift für Kristallographie - New Crystal Structures 214 (1999) 447–448; doi:10.1515/ncrs-1999-0423

data_8101635
_publ_section_title
;
Crystal structure of dilithium (nitridolithiate/ferrate(I)), Li~2~
[(Li~1-x~Fe~x~)N], x = 0.63
;
_journal_coden_ASTM              ZKNSFT
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              447
_journal_page_last               448
_journal_paper_doi               10.1515/ncrs-1999-0423
_journal_volume                  214
_journal_year                    1999
_chemical_formula_moiety         'Li2[(Li1-xFex)N] x=0.63'
_chemical_formula_structural     'Li2 [(Li1-x Fex) N] x=0.63'
_chemical_formula_sum            'Fe0.63 Li2.37 N'
_chemical_formula_weight         64.18
_space_group_IT_number           191
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   3.724(2)
_cell_length_b                   3.724(2)
_cell_length_c                   3.6297(10)
_cell_measurement_temperature    293(2)
_cell_volume                     43.60(4)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    2.444
_refine_ls_R_factor_obs          0.0297
_refine_ls_wR_factor_obs         0.0725
_cod_database_code               8101635
Crystal structure of dicalcium (dinitridolithiate/ferrate(I)), Ca~2~{Li[(Li~1-x~Fe~x~)N~2~]}, x = 0.82
Klatyk, Jens; Kniep, Rüdiger; Zeitschrift für Kristallographie - New Crystal Structures 214 (1999) 451–452; doi:10.1515/ncrs-1999-0425

data_8101636
_publ_section_title
;
 Crystal structure of dicalcium (dinitridolithiate/ferrate(I)),
 Ca~2~{Li[(Li~1-x~Fe~x~)N~2~]}, x = 0.82
;
_journal_coden_ASTM              ZKNSFT
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              451
_journal_page_last               452
_journal_paper_doi               10.1515/ncrs-1999-0425
_journal_volume                  214
_journal_year                    1999
_chemical_formula_moiety         'Ca2 {Li [(Li0.19 Fe0.82) N2]}'
_chemical_formula_structural     'Ca2 {Li [(Li0.19 Fe0.82) N2]}'
_chemical_formula_sum            'Ca4 Fe0.82 Li1.18 N2'
_chemical_formula_weight         162.17
_space_group_IT_number           136
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      136
_symmetry_space_group_name_Hall  '-P 4n 2n'
_symmetry_space_group_name_H-M   'P 42/m n m'
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   5.3559(8)
_cell_length_b                   5.3559(8)
_cell_length_c                   6.6778(12)
_cell_measurement_temperature    293(2)
_cell_volume                     191.56(5)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    2.964
_refine_ls_R_factor_obs          0.0313
_refine_ls_wR_factor_obs         0.0673
_cod_database_code               8101636
Crystal structure of dilithium (nitridolithiate/manganate(I)), Li~2~[(Li~1-x~Mn~x~)N], x = 0.73
Klatyk, Jens; Kniep, Rüdiger; Zeitschrift für Kristallographie - New Crystal Structures 214 (1999) 445–446; doi:10.1515/ncrs-1999-0422

data_8101637
_publ_section_title
;
 Crystal structure of dilithium (nitridolithiate/manganate(I)),
 Li~2~[(Li~1-x~Mn~x~)N], x = 0.73
;
_journal_coden_ASTM              ZKNSFT
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              445
_journal_page_last               446
_journal_paper_doi               10.1515/ncrs-1999-0422
_journal_volume                  214
_journal_year                    1999
_chemical_formula_moiety         'Li2[(Li1-xMnx)N] x=0.73'
_chemical_formula_structural     'Li2 [(Li1-x Mnx) N] x=0.73'
_chemical_formula_sum            'Li2.27 Mn0.73 N'
_chemical_formula_weight         69.87
_space_group_IT_number           191
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      191
_symmetry_space_group_name_Hall  '-P 6 2'
_symmetry_space_group_name_H-M   'P 6/m m m'
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   3.7263(4)
_cell_length_b                   3.7263(4)
_cell_length_c                   3.8281(4)
_cell_measurement_temperature    293(2)
_cell_volume                     46.033(8)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    2.520
_refine_ls_R_factor_obs          0.0249
_refine_ls_wR_factor_obs         0.0629
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Hexagonal' changed to 'hexagonal'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_database_code               8101637
Crystal structure of dimeric aqua(<i>N</i>-salicylidene-<i>rac</i>- alaninato)copper(II) monohydrate, C~10~H~11~CuNO~4~ · H~2~O
Warda, Salam A.; Zeitschrift für Kristallographie - New Crystal Structures 213 (1998) 771–772; doi:

data_8101638
_publ_section_title
;
Crystal structure of dimeric aqua(<i>N</i>-salicylidene-<i>rac</i>-
alaninato)copper(II) monohydrate, C~10~H~11~CuNO~4~ &#x00B7; H~2~O
;
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              771
_journal_page_last               772
_journal_volume                  213
_journal_year                    1998
_chemical_formula_sum            'C10 H13 Cu N O5'
_chemical_formula_weight         290.75
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90.00
_cell_angle_beta                 100.359(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   7.7618(4)
_cell_length_b                   9.9276(3)
_cell_length_c                   15.1889(5)
_cell_measurement_temperature    293(2)
_cell_volume                     1151.32(8)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    1.677
_refine_ls_R_factor_obs          0.0476
_refine_ls_wR_factor_obs         0.1310
_cod_depositor_comments
;
The following automatic conversions were performed:
'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to '/home/saulius/struct/CIF-dictionaries/cif_core.dic'
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_enum 1527 2010-12-29 10:47:43Z saulius 
;
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               8101638
Crystal structure of strontium dihydrogenphosphate, Sr(H~2~PO~4~)~2~
Königstein, Dagmar; Jansen, Martin; Zeitschrift für Kristallographie - New Crystal Structures 213 (1998) 696–696; doi:

data_8101639
_publ_section_title
;
Crystal structure of strontium dihydrogenphosphate, Sr(H~2~PO~4~)~2~
;
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              696
_journal_page_last               696
_journal_volume                  213
_journal_year                    1998
_chemical_formula_analytical     'Sr1 P2 O8 H4'
_chemical_formula_structural     'Sr (H2 P O4)2'
_chemical_formula_sum            'H4 O8 P2 Sr'
_chemical_formula_weight         281.59
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                103.98(2)
_cell_angle_beta                 96.97(2)
_cell_angle_gamma                109.70(2)
_cell_formula_units_Z            2
_cell_length_a                   6.7455(10)
_cell_length_b                   7.0833(10)
_cell_length_c                   7.8019(10)
_cell_measurement_temperature    293(2)
_cell_volume                     332.07(8)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    2.816
_refine_ls_R_factor_obs          0.0398
_refine_ls_wR_factor_obs         0.0978
_cod_database_code               8101639
Crystal structure of barium heptachloroeuropate(III), Ba~2~[EuCl~7~]
Masselmann, Sönke; Meyer, Gerd; Zeitschrift für Kristallographie - New Crystal Structures 213 (1998) 690–690; doi:

data_8101640
_publ_section_title
;
Crystal structure of barium heptachloroeuropate(III), Ba~2~[EuCl~7~]
;
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              690
_journal_page_last               690
_journal_volume                  213
_journal_year                    1998
_chemical_formula_sum            'Ba2 Cl7 Eu'
_chemical_formula_weight         674.79
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90.00
_cell_angle_beta                 90.674(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   6.8164(7)
_cell_length_b                   15.5896(15)
_cell_length_c                   10.5431(10)
_cell_measurement_temperature    293(2)
_cell_volume                     1120.3(2)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    4.001
_refine_ls_R_factor_obs          0.0300
_refine_ls_wR_factor_obs         0.0680
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' tag value 'monocline' was replaced with
'monoclinic' value.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_database_code               8101640
Crystal structure of <i>cis</i>-dichloro(metforminuro)gold(III) dimethylacetamide, C~16~H~38~Au~2~Cl~4~N~12~O~2~
Lemoine, Pascale; Viossat, Bernard; Nguyen-Huy, Dung; Zeitschrift für Kristallographie - New Crystal Structures 213 (1998) 726–728; doi:

data_8101641
_publ_section_title
;Crystal structure of <i>cis</i>-dichloro(metforminuro)gold(III)
 dimethylacetamide, C~16~H~38~Au~2~Cl~4~N~12~O~2~
;
_journal_issue                   4
_journal_name_full
'Zeitschrift f\"ur Kristallographie - New Crystal Structures'
_journal_page_first              726
_journal_page_last               728
_journal_volume                  213
_journal_year                    1998
_chemical_formula_sum            'C16 H38 Au2 Cl4 N12 O2'
_chemical_formula_weight         966.32
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                93.83(5)
_cell_angle_beta                 95.61(3)
_cell_angle_gamma                97.69(5)
_cell_formula_units_Z            2
_cell_length_a                   8.838(4)
_cell_length_b                   13.102(9)
_cell_length_c                   13.388(5)
_cell_measurement_temperature    293(2)
_cell_volume                     1523.9(14)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    2.106
_exptl_crystal_density_meas      2.07
_refine_ls_R_factor_obs          0.0594
_refine_ls_wR_factor_obs         0.1295
_cod_database_code               8101641